Preparation and Properties of Epoxy Resin-Coated Micro-Sized Ferrosilicon Powder
Jiangang Kua*, Huihuang Chenb, Kui Hea, Quanxiang Yana
aCollege of Zijin Mining, Fuzhou University, Fuzhou 350116, Fujian, China
bSchool of Chemical Engineering, University of Queensland, St. Lucia, Brisbane, QLD 4072, Australia
Received: October 27, 2015; Revised: February 3, 2016; Accepted: June 13, 2016
Ferrosilicon powder surface coated with a dense epoxy resin membrane was prepared via coating
precipitation methods using silane coupling agents as the modiier and epoxy resin as the coating agent.
FTIR, FESEM, MPMS-XL, and TG-DSC were used to analyze the morphology, surface composition,
magnetic property and thermostability of ferrosilicon powder before and after the modiication and coating. The experimental results indicate that epoxy resin membranes of a certain thickness were
successfully coated onto the surface of ferrosilicon powder; coatings of epoxy resin contributed to the decreased the rate of weight loss via the reduced wear of the coatings and provided resistance to corrosion; the apparent viscosity of medium suspension with coated ferrosilicon was smaller than
that of magnetite. Meanwhile, analysis reveals that room-temperature magnetic hysteresis loops of ferrosilicon powder remain basically unchanged before and after coating.
Keywords: ferrosilicon powder, epoxy resin coating, viscosity, magnetic hysteresis loops, oxidation resistibility
Heavy liquids and/or heavy suspensions with densities between those of valuable minerals and gangue minerals are adopted as the media to achieve the objective of separation in the dense medium separation (DMS) process1. DMS includes
heavy–luid separation and suspension liquid separation. Weighting agents, which are particularly important as a kind
of suspension liquid separators, were used in heavy medium separationby Blezard et al.2 and Bradbury et al.3 respectively. DMS is a process whereby particles are sorted primarily on the
basis of their densities. Particles with a wide range of densities are introduced into a medium suspension of a given density. Those particles that are lighter than the medium density rise. These are commonly referred to as loats. The particles that are heavier than the medium density sink, and these are commonly referred to as sinks4. In industrial production, considering the required separating density, viscosity and stability of the system, the selected weighting agents should have high density, be
diicult to make muddy and to oxidize, and be easy to recycle5. In principle, media with a density higher than that of water can be used as the weighting agents6. Currently, the commonly used weighting agents in industry are magnetite, ferrosilicon, ilmenite, barite, pyrite and industrial waste, such as reduced iron and magnetic beads, which were industrially used by Hamidreza
et al.7 and experimentally used by Ramadan et al.8 respectively. Magnetite is widely used in dense medium coal separation due
to its low cost. However, magnetite has the following limitations compared with ferrosilicon. First, it is diicult to control the
particle–size distribution of magnetite powder, which results in the huge reduction of density distribution uniformity of the suspension system, which is one of the most important technical indicators for DMS9. Second, the rheological properties of the suspension system prepared by magnetite powder are poor
because magnetite powder is nonspherical. The τ values and η values of the suspension systems prepared using magnetite
powder are far greater than those prepared using ferrosilicon
powder under the same system density (above 2.34 g/cm3)10,11. Third, magnetite has edges and corners; as a result, suspension systems prepared using magnetite will intensify the wear of the pipelines and equipment12, 13. Fourth, magnetite powder is brittle, and the number of coarse particles will decrease because of the wear and tear14. Correspondingly, the number
of ine particles will increase. Hence, it is diicult to achieve
the automatic control of the density of the suspension system15.
Fifth, the density of magnetite (approximately 4.2 g/cm3) is smaller than that of ferrosilicon; therefore, more magnetite will be required to prepare a suspension system of the same density
with respect to ferrosilicon.
However, the poor antioxidant capacity and high price
limit the application range of ferrosilicon. Speciically, spray
ferrosilicon of high density is easy to oxidize in aqueous solutions, and the presence of carbon impurities will enhance the oxidization rate, resulting in faster wear16. Therefore, understanding how to improve the antioxidant capacity is
of crucial importance.
In this paper, the preparation of epoxy resin-coated
ferrosilicon powder is described. The antioxidant capacity
of such powder is studied using FTIR and FE–SEM, and the room–temperature magnetic hysteresis loops and
thermostability before and after modiication are analyzed by MPMS–XL and TG–DSC, respectively.
2. Experimental Section
2.1. Materials and reagents
The epoxy resin 618 and epoxy resin curing agent 5618
were obtained from Shanghai Resin Factory Co., Ltd. (Shanghai,
China). The epoxy resin 618 is a kind of bisphenol A-type epoxy resin with the Epoxy value 0.51~0.54eq/100g and the curing agent 5618 is a modiied aliphatic amine containing aromatic ring adduct containing 260-300 mgKOH/g amine.
The KH–550 silane coupling agent was obtained from Beijing Shenda Fine Chemical Company (Beijing, China); its structure is:
Eighty milliliters of absolute ethanol was blended with
3.0 g of a mixture of epoxy resin, epoxy resin curing
agent and ferrosilicon particles pretreated with ultrasonic
in ethanol for 15 min. Next, the pretreated ferrosilicon
particles was placed into the hydrolysate and stirred for 3 h, after which ferrosilicon powder was separated by
iltration, washed by deionized water three times, and then dried and solidiied at 100 ℃ in a vacuum drying
oven for 1 h. The steps described above were repeated to
obtain epoxy resin-coated ferrosilicon powder for coating
times higher than 10.
3. Results and Discussion
3.1. Efect of coating times on the morphology
of epoxy resin-coated ferrosilicon powder
determined by analysis of FE–SEM images
The coating times and morphology of epoxy
resin-coated ferrosilicon powder are shown in Figure 1. The
surface morphologies of the bare and the coated ferrosilicon
powder with diferent coating times and magniications are shown. Ferrosilicon particles share the characteristics of an irregular drop shape and basically take the form of
spheres with relatively smooth and non–concave/convex
surfaces. Furthermore, the degree of sphericity of coated ferrosilicon particles with diferent coating times almost remains unchanged compared to that of the uncoated particles.
However, the surface smoothness decreases with decreasing coating times, especially when the coating times are higher
than 25. Hence, all further experiments were performed with coating times of 25.
The reagent-grade ethyl alcohol (alcohol content: 99.7%) was obtained from Tianjin Jinhuitaiya Chemical Reagent Co., Ltd. (Tianjin, China). The soft magnetic metal powder of ferrosilicon (nitrogen atomized powder, Fe 92~93, Si 5~6, Cr 1~2, and other impurities less than 0.1 wt.%, density 7.35
g/cm3) was obtained from Changsha Tianjiu Metal Materials
Co., Ltd. (Changsha, China). The deionized water used in the experiment was lab–made.
2.2. Analysis and characterization
An infrared spectrometer, Nicolet 380, was used to
study the FTIR spectra of ferrosilicon particles to determine whether new chemical bonds are generated before and after
modiication via silane coupling agent and coating with epoxy resin and to further analyze the efects of modiication and coating. A Nova NanoSEM 230 model Scanning Electron
Microscope was used to analyze the morphology and
coating thickness of the epoxy resin-coated ferrosilicon powder. MPMS (SQUID)–XL measurement was carried
out to determine the magnetic property before and after the
modiication and coating. A simultaneous thermal analyzer Netzsch STA449C was used to analyze the antioxidation capacity of ferrosilicon powder before and after coating. All
other experimental equipment used included an electronic analytic balance BSA822, a precise timing electric mixer JJ–1, an ultrasonoscope VGT–1730TD, a thermostatic water
bath DF–101S and a vacuum drying oven DZF–6020.
The pretreatment experiments were irst performed by taking 5 g of ferrosilicon powder (1.25±0.074 mm) into a
certain volume of ethanol medium for ultrasonic treatment
for 15 min to obtain the pretreated ferrosilicon powder.
Then, 80 ml of absolute ethanol, 5 ml of deionized water,
and 2.0 g of silane coupling agent were collected, blended and stirred at low stirring speed for 0.5 h for the hydrolysis of silane coupling agent. Next, the pretreated ferrosilicon powder was placed into the hydrolysate and immersed for 0.5 h. Subsequently, 1.5 g of mixture of epoxy resin and epoxy
resin curing agent was placed into the above solutions, stirred
for 3 h, and then separated by iltration, followed by washing by deionized water three times. The mixture was then dried and solidiied at 100 ℃ in a vacuum drying oven for 1 h.
After layer–by–layer coated for 10 times according to
the above procedure, the following procedure was used.
Figure 2 shows that the thickness of the epoxy resin
coated onto the ferrosilicon powder surface increases with
the increase in the coating times. In addition, the cross–
sectional images (Figure 1) at high resolution demonstrate that epoxy resin membranes coated onto the ferrosilicon powder surface are smooth and have a compact structure
without holes and stratiication phenomenon, which indicates
that chemical reactions occurred between layers of epoxy resin and that the layers of epoxy resin were held together
by chemical bonds.
Figure 2: Relationship between the thicknesses of the epoxy resin and the number of coatings
Figure 2 shows that the thickness of the epoxy resin
coated onto the ferrosilicon surface increases linearly with
increasing coating times. Speciically, the mean thickness of the epoxy resin ilm increases 15 nm with each coating.
3.2. Efect of modiication and coating on the FTIR
spectra of the ferrosilicon particles
FTIR spectra (background corrected) of ferrosilicon particles before and after modiication and coating are shown in Figure 3. As observed in the FTIR spectra, peaks at 3435
cm–1 and 1634 cm–1 attributed to O–H stretching vibration
and lexural vibration, respectively, are associated with the constitution water and the free water. The peak at 1457 cm–1
in the FTIR spectra of the modiied ferrosilicon particles by
the silane coupling agent results from the generated silanol
(NH2(CH2)3SiOH). The bands between 1450 cm−1 and 1350 cm−1 are attributed to the deformation vibrations of –CH2. The bands at 1100 cm−1 and 460 cm–1 are attributed to the
Si–O–Si antisymmetric stretching vibration and lexural
vibration, respectively, which demonstrates that a chemical
reaction occurred during the modiication. The band at 1560
cm–1 in the FTIR spectra of coated ferrosilicon particles results
from the C–N stretching vibration, the band at 1200 cm–1 corresponds to the C–C antisymmetric stretching vibration, and the bands in the range from 800 to 860 cm–1 are attributed to bending vibration adsorption of two adjacent H atoms of the opposite–substituted benzene ring, indicating that the surface of the coated ferrosilicon particles is covered
by epoxy resin.
Through the analysis, the modiication mechanism of
ferrosilicon particles by the silane coupling agent can be
Figure 3: FTIR spectra of the ferrosilicon particles: (a) unmodiied, (b) modiied–coated, and (c) modiied
concluded: irst, hydrolysis of (–OCH2CH3)3 generates silanol
(NH2(CH2)3SiOH) when the carbonyl of the silane coupling agent KH–550 encounters hydroxy created by water near the
surface of the ferrosilicon particles. Next, hydrogen bonds
between part of the silanol and the carbonyl near the surface of the ferrosilicon particles form or further condense to form
Si–O–Fe. Meanwhile, the silanol groups of the silane coupling
agent interact to produce a condensation product to form the
net structure on the surface of ferrosilicon particles. There is a large amount of–NH2 groups in the KH–550 modiied ferrosilicon particles that can react with the epoxy groups
of 618 epoxy resin to form epoxy resin membranes.
3.3. Magnetic property measurement
Room–temperature magnetic hysteresis loops of ferrosilicon
particles before and after modiication and coating are shown in Figure 4. The magnetic hysteresis loops of three types of ferrosilicon particles (unmodiied, modiied and coated)
are narrow and smooth and share the single soft magnetic
property. Additionally, the coercivity and remanence of ferrosilicon particles before and after modiication almost
remained the same, and only the coercivity and the remanence
of the coated ferrosilicon particles decreased 0.3%, which is partially due to the presence of the epoxy resin coating.
In conclusion, magnetic hysteresis loops of ferrosilicon particles almost remain unchanged before and after coating, and its magnetic properties remained intact17.
3.4. hermostability measurement
Simultaneous thermogravimetry (TG) and diferential
scanning calorimetry (DSC) experiments were carried out
before and after coating with epoxy resin using a Netzsch
STA 449 C Jupiter at a heating rate of 10 ℃ min−1. The
results are shown in Figure 5.
As observed from Figure 5(a), the irst highest anodic peak
of TG curve resulted from the oxidation (an exothermic process) of iron due to the formation of an iron–carbon primary battery on the surface of the ferrosilicon particles18, with the weight
Figure 4: Room–temperature magnetic hysteresis loops of ferrosilicon particles
Figure 5: TG–DSC curves of ferrosilicon particles: (a) uncoated (b) coated water on the surface of the ferrosilicon particles occurred,
with a weight loss corresponding to a wide adsorption peak which can be seen from DSC curve. TG reveals the course
of the weight loss at 180 ℃ resulting from the oxidation of
carbon. As all of the above-mentioned processes occur at
the surface of ferrosilicon particles, the change in the DSC
curve is attributed to the endothermic reaction.
According to Figure 5(b), there is an adsorption peak at
40 ℃ in the DSC curve of the coated ferrosilicon particles resulting from the evaporation of adsorbed water on the
surface of ferrosilicon particles along with the weight loss.
At 250 ℃, an obvious adsorption peak existed with weight loss, which resulted from the structural damage of the epoxy
resin. The weight leveled of after 280 ℃ because the structure
of epoxy resin was completely destroyed. It is clear that the
antioxidant capacity of iron in the coated ferrosilicon particles
was improved as no oxidation exothermic peak of iron is observed in the DSC curve of coated ferrosilicon particles.
3.5. Wear resistance measurement
The wear resistance experiment of coated ferrosilicon particles was performed in an Agitator (IKA RW20 mixer) as a function of time to determine the corrosion resistance
ability of coated FeSi particles. The density of used ferrosilicon suspensions with tap water is 3.0 kg/l. And the
stirring rate is kept constant during the experiment. Under
given time intervals, coated ferrosilicon particle is sampled
and characterized by SEM technique. Results are shown in Figure 6.
It is obvious from Figure 6(a) and Figure 6(b) that
FeSi particles are still coated completely after 8 h stirring.
However, corrosion of coated FeSi particles happens after
9h (Figure 6(c)). This is consistent with the weight loss rate results. The weight loss of the coated sample is only negligible 0.03% in the irst 8 h (Figure 6(d)). Thereafter, weight loss dramatically increases up to around 3% after 9 h. This demonstrates that the coating is quite stable and resistant to corrosion in the irst 8 h. However, corrosion occurs when the stirring time is longer than 9 h.
3.6. Viscosity measurement
Two samples of coated ferrosilicon particles and magnetite
were used in the tests. The magnetite (assayed at 71.3% Fe and 1.1% SiO2 with the density 5.0 kg/m
3) provided by the
Makeng Mining Co., Ltd. (Fujian, China) was studied as a comparison. Prior to laboratory experiments the samples were
analyzed using an OMEC Sample Analyzer (LS-CWMⅢ)
to deine their size ranges. It can be seen in Figure 7 that the
average size of ferrosilicon and magnetite is similar, which
is 76.3 and 75.8 (Dav/μm), respectively. It is also observed that the particle size distribution of magnetite is broader
than that of ferrosilicon.
Since the measurements were carried out to study the
efect of viscosity of the diferent suspensions used as dense
medium in gravity separation, tap water was utilized in
measurements. As known, the samples are magnetic and
remnant magnetic forces cause aggregation that may strongly
afect the viscosity measurements. In order to reduce the
negative impact and obtain good reproducibility, high-speed
blending was applied to prepare the suspensions.
The viscosity tests of diferent suspensions were carried out using Brookield DV-Ⅱ Pro viscosimeter with ultra-low
viscosity adapter at room temperature (23.6 ℃). The results are shown in Figure 8.
It is obvious from Figure 8 that the apparent viscosity of ferrosilicon suspension is smaller than that of magnetite in
increases slowly when the medium density is from 1.2 to 2.2 kg/l and then increases quickly along with the increase of the medium density.
There are many advantages of coated ferrosilicon
powders in practical applications. First, it is easy to control
the particle–size distribution of coated ferrosilicon powders, which is one of the most important technical indicators for DMS19. Second, the rheological property of the suspension system prepared by coated ferrosilicon powders with high sphericity is good for accelerating the DMS process because
the τ and η values of the suspension systems are far lower
than those of the other suspension systems under the same
density (especially a density above 2.34 g/cm3)20. Third, the wear and tear of pipelines and equipment will decrease sharply with the use of coated ferrosilicon powder with high sphericity21. Fourth, the particle size characteristics of the suspension system will not change much because the wear resistance of the coated ferrosilicon powders will be greatly
increased. Hence, it is easy to achieve automatic control of the density of the suspension system.
In brief, the suspension system prepared by coated ferrosilicon powders has many advantages, such as high
density, high stability, good luidity, good durability, and ease of control. Therefore, the applications of coated ferrosilicon
powders will continue to expand with the development of
the technology. Because the epoxy resin-coated ferrosilicon
powders are mainly used in ambient atmosphere, preventing the oxidation of iron and reducing the wear rate in water
are the best ways to increase the working life of ferrosilicon particles. Thus, the as–prepared ferrosilicon particles coated by epoxy resin can expect to address this issue.
In this paper, ferrosilicon powder coated with a dense epoxy resin membrane was obtained via heterogeneous Figure 6: Efect of stirring time on residual weight of coated
ferrosilicon particles. SEM micrographs of (a) t = 0 h, (b) t = 3 h and (c) t = 9 h.
Figure 7: Particle size ranges determined for the coated ferrosilicon particles and magnetite
Figure 8: (a) Efect of medium composition on apparent viscosity. (b) Selected zone of (a). important role in the apparent viscosity of two suspensions,
precipitation coating methods using silane coupling agents
as the modiier and epoxy resin as the coating agent. The thickness of ferrosilicon particles increases by
approximately 10 nm after each coating, and ferrosilicon particles remain spherical after coating 20 times, without
aggregation among particles. The FT–IR results reveal that coating of the silane coupling agent KH550-modiied ferrosilicon particles by epoxy resin is attributed to chemisorption.
The experimental results indicate that epoxy resin
membranes of a certain thickness were successfully coated
onto the surface of ferrosilicon powder; coatings of epoxy resin contributed to the decreased the rate of weight loss via the reduced wear of the coatings and provided resistance to corrosion; the apparent viscosity of medium suspension
with coated ferrosilicon was smaller than that of magnetite.
Meanwhile, analysis reveals that room-temperature magnetic hysteresis loops of ferrosilicon powder remain basically
unchanged before and after coating.
This work was supported by the National Natural Science Foundation of China (Grant No. 51104048), for which the authors express their appreciation.
1. Law HS, Masliyah JH, Mac Taggart RS, Nandakumar K. Gravity separation of bidisperse suspensions: Light and heavy particle species. Chemical Engineering Science. 1987;42(7):1527-1538.
2. Blezard M, Grover BW, Messenger ET, Nicholson WJ, Williams MJ, inventors. Albright & Wilson Limited, assignee. Functional
luids and liquid cleaning compositions and suspending media. US Patent 5,807,810. 1998 Sep 15.
3. Bradbury A, Sawdon CA, inventors. M-I LLC, assignee. Additive
for increasing the density of a luid and luid comprising such
additive. US Patent 6,586,372. 2003 Jul 1.
4. Gupta A, Yan DS. Mineral processing design and operation: an introduction. Amsterdam: Elsevier Science; 2006.
5. Bosman J. The art and science of dense medium selection. Journal of the Southern African Institute of Mining and Metallurgy.
6. Waanders FB, Rabatho JP. Recovery of heavy minerals by means of ferrosilicon dense medium separation material. In: Mercader RC, Gancedo JR, Cabral Prieto A, Baggio-Saitovitch E, eds.
LACAME 2004 Proceedings of the 9th Latin American Conference
on the Applications of the Mössbauer Efect (LACAME 2004)
held in Mexico City, Mexico, 19–24 September 2004. Berlin
Heidelberg: Springer; 2005. p. 55-60.
7. Habetinejad H, Jorjani E, Sam A. Evaluation of Mayer curve validity on feed blending at the Zarand coal washery plant.
International Journal of Mining Science and Technology.
8. Ramadan Q, Samper V, Poenar DP, Yu C. An integrated microluidic platform for magnetic microbeads separation and coninement.
Biosensors and Bioelectronics. 2006;21(9):1693-1702.
9. He YB, Laskowski JS, Klein B. Particle movement in non-Newtonian slurries: the efect of yield stress on dense medium separation.
Chemical Engineering Science. 2001;56(9):2991-2998.
10. Bevilacqua P, De Lorenzi L, Ferrara G. Rheology of low density suspensions in dense medium separation of post-consumer plastics. Coal Preparation. 2000;21(2):197-209.
11. Mabuza NT, Pocock J, Loveday BK. The use of surface active chemicals in heavy medium viscosity reduction. Minerals Engineering. 2005;18(1):25-31.
12. Cavenati S. Grande CA, Rodrigues AE. Upgrade of methane from landill gas by pressure swing adsorption. Energy & Fuels.
13. Chu KW, Kuang SB, Yu AB, Vince A, Barnett GD, Barnett PJ. Prediction of wear and its efect on the multiphase low and separation performance of dense medium cyclone. Minerals Engineering. 2014;56:91-101.
14. Golden DC, Ming DW, Morris RV, Brearley AJ, Lauer HV, Treiman AH, et al. Evidence for exclusively inorganic formation of magnetite in Martian meteorite ALH84001. American Mineralogist. 2004;89(5-6):681-695.
15. Zhao ZY, Fan ZH, Zhang JJ, Xia ZQ. Research on ride comfort of nonlinear vehicle suspension. Advanced Materials Research.
16. Østensen OJ. Upgrading of–grades from the silicon process:
Increasing the silicon yield from Elkem Thamshavn using mechanical or metallurgical separation. [Master Dissertation]; Trondheim: Institutt for materialteknologi NTNU; 2011. 17. Dong D, Guan J, Wang W, Li W, Zhou J. Preparation
and electromagnetic properties of micrometer Fe flakes modified with epoxy resin. Acta Metallurgica Sinica.
18. Narayan S. Rajeshkannan A. Strain hardening behaviour in forming of sintered iron-0.35% carbon powder metallurgy preform during cold upsetting. Materials Research.
19. Dworzanowski M. Optimizing the performance of wet drum magnetic separators. Journal of the Southern African Institute of Mining and Metallurgy. 2010;110(11):643-653.
20. Klein B. Rheology and stability of magnetite dense media [PhD Thesis]. Vancouver: University of British Columbia; 1992. 21. Red’kina NI, Khodakov GS, Gorlov EG. Coal fuel slurry
for internal combustion engines. Solid Fuel Chemistry.